Research Article  Open Access
Enriched ElementFree Galerkin Method for Fracture Analysis of Functionally Graded Piezoelectric Materials
Abstract
A new method using the enriched elementfree Galerkin method (EEFGM) to model functionally graded piezoelectric materials (FGPMs) with cracks was presented. To improve the solution accuracy, extended terms were introduced into the approximation function of the conventional elementfree Galerkin method (EFGM) to describe the displacement and electric fields near the crack. Compared with the conventional EFGM, the new approach requires smaller domain to describe the cracktip singular field. Additionally, the domain of the nodes was not affected by the crack. Therefore, the visibility method and the diffraction method were no longer needed. The mechanical response of FGPM was discussed, when its material parameters changed exponentially in a certain direction. The modified integrals for FGPM were deduced, whose results were compared with the results of the conventional EFGM and the analytical solution. Numerical example results illustrated that this method is feasible and precise.
1. Introduction
Functionally graded materials (FGMs) are composite materials formed of two or more constituent phases with a continuously variable composition. During design, the requirements of structural strength, reliability, and lifetime of piezoelectric structures/components call for enhanced mechanical performance, including stress and deformation distribution under multifield loading. In recent years, the emergence of FGMs has demonstrated that they have the potential to reduce stress concentration and to provide improved residual stress distribution, enhanced thermal properties, and higher fracture toughness. Consequently, a new kind of material, functionally graded piezoelectric materials (FGPMs), has been developed to improve the reliability of piezoelectric structures by introducing the concept of the wellknown FGM to piezoelectric materials [1].
At present, FGPMs are usually associated with particulate composites where the volume fraction of particles varies in one or several directions. One of the advantages of a monotonous variation of volume fraction of constituent phases is elimination of the stress discontinuities that are often encountered in laminated composites and accordingly avoidance of delaminationrelated problems. How all these aspects can be improved and what the mechanisms might be are popular topics which have received much attention from researchers. Wang and Noda [2] investigated the thermally induced fracture of a functionally graded piezoelectric layer bonded to a metal. Ueda studied the fracture of an FGPM strip with a normal crack [3, 4], a symmetrical FGPM strip with a center crack [5], and an FGPM strip with a twodimensional crack [6, 7]. Li and Weng [8] solved the problem of an FGPM strip containing a finite crack normal to boundary surfaces. Hu et al. [9] studied the problem of a crack located in a functionally graded piezoelectric interlayer between two dissimilar homogenous piezoelectric half planes. Rao and Kuna [10] presented an interaction integral method for computing stress intensity factors (SIFs) and the electric displacement intensity factor (EDIF) in FGPM under thermoelectromechanical loading. Borrelli et al. [11] used the energydecay inequality technique to analyze the decay behavior of end effects in antiplane shear deformation in piezoelectric solids and FGPMs. Zhong and Shang [12] developed an exact solution for a functionally graded piezothermoelectric rectangular plate. Dai et al. [13] conducted a theoretical study of electromagnetoelastic behavior for an FGPM cylinder and sphere. They then extended their solutions to include thermal effects [14]. Zhong and Yu [15] analyzed the FGPM beam with arbitrarily graded material properties along the beam thickness direction. Based on the layerwise finite element model, Shakeri and Mirzaeifar [16] performed a static and dynamic analysis of a thick FGM plate with piezoelectric layers. Wang et al. [17] analytically investigated the axisymmetric bending of circular plates whose material properties varied with the thickness. Using the Fourier transform technique, Chue and Yeh [18] developed a system of singular integral equations for angle cracks in two bonded FGPMs under antiplane shear. Chen and Bian [19] studied the wave propagation characteristics of an axially polarized, functionally graded, piezoceramic cylindrical transducer submerged in an infinite fluid medium. Ueda [20] addressed the problem of two coplanar cracks in an FGPM strip under transient thermal loading. Ben Salah et al. [21] examined the propagation of ultrasonic guided waves in FGPMs. Wang et al. [22] studied the singularity behavior of electroelastic fields in a wedge with angularly graded piezoelectric material (AGPM) under antiplane deformation. Chue and Yeh [23] extended the results of the case of two arbitrarily oriented cracks in two bonded FGM strips.
In the field of engineering technology, accurate solutions computed with analytic methods are only available in problems with relatively simple equations and regular geometry. As for most problems, especially in the case of complex engineering, analytic solutions cannot be computed. Therefore, research has been going on for many years that has led to the development of another approach—the numerical method. With the rapid development and wide application of computers, numerical analysis and theoretical investigation and experimental investigation are considered as the three major research approaches. As one of the most effective tools for the study of mechanics, the finite element and other numerical methods have been widely used in scientific research and engineering practice. FEM analysis of piezoelectric structures with a crack under dynamic electromechanical loading was presented by Enderlein et al. [24]. A survey on numerical algorithms for crack analyses in piezoelectric structures to be used with FEM for determining fracture parameters was presented by Kuna [25]. Béchet et al. [26] presented an application of XFEM to the analysis of fracture in piezoelectric materials. Nanthakumar et al. [27] analyzed the multiple flaws in piezoelectric structures using XFEM and level sets. Sharma et al. [28] analyzed a subinterface crack in piezoelectric bimaterials with XFEM. Bouvier et al. [29] studied the inverse problems in structural analysis: application to atherosclerotic plaque elasticity reconstruction by using the XFEM.
Compared with the extended finite element method, however, elementfree method has a unique feature in solving the problems of crack growth, plastic flow of materials, geometric distortion and phase transition, and singularity. The notable feature of this method is that, in establishing the discrete equation, it does not need mesh but only needs to arrange discrete points in the global domain. Thus, it not only avoids the complicated process of mesh formation, but also greatly reduces the influence of mesh distortion. Various meshless methods have been applied to the analysis of smart materials and structures such as the meshless point collocation method (PCM) [30], the point interpolation meshfree method (PIM) [31], a novel truly hybrid meshlessdifferential order reduction method (hMDOR) [32], and the local PetrovGalerkin method (MLPG) [33]. Among these meshless methods, the elementfree Galerkin method (EFGM) [34], developed by Belytschko et al., has good compatibility and stability and will not have the problem of shear locking of volume even in adopting linear primary function. And fast convergence speed and high accuracy can be achieved. EFGM was widely applied in fracture mechanics. Rabczuk and Belytschko analyzed the problem of a threedimensional large deformation meshfree method for arbitrary evolving cracks [35]. Rabczuk et al. deduced a simplified meshfree method for shear bands with cohesive surfaces [36].
In this study, a type of electromechanicalcoupling enriched elementfree Galerkin method based on the enriched EFG methods [37, 38] is developed. Enriched terms were introduced into the approximation function of the conventional EFGM to describe the displacement and electric fields near the crack. Compared with the conventional EFGM, this method only needs a small domain to describe the cracktip singular field. Furthermore, the domain of the node is not affected by the crack without using the visibility method and diffraction methods.
2. Basic Equations for TwoDimensional FGPM
The governing equations and the boundary conditions of FGPM are briefly given.
Constitutive Equations. Considerin which , , and are the elastic, piezoelectric, and dielectric constants, respectively. , , , and are the stress tensor, strain tensor, electric field, and electrical displacements.
Strains are related to displacements by the expressionwhere and are, respectively, the displacements in  and directions.
The electric field is related to the electric potential by the expression
Types of Gradation. The properties of FGM are usually assumed to have the same functions of certain space coordinates. Exponential material gradation is commonly used graded forms.
All the material constants including elastic constants, piezoelectric parameters, and dielectric constants follow the exponential law:where represents material constants such as , , or , is the corresponding value at the plane , and α denotes a material graded parameter.
The field equations of electroelasticity are reduced to twodimensional form in the special cases: plane strain. Considering a transversely isotropic FGPM, according to (1), the  plane is the isotropic plane, and one can employ either the  or  plane for the study of plane electromechanical phenomena. The plane strain conditions require thatBy substitution of (10) into (1), we haveor inverselywhere , , and are the reduced material constants. They are related to the elastic compliance tensor , the piezoelectric tensor , and the dielectric impermeability tensor by the following relations [39]:
Boundary Conditions. In electroelasticity theory, mechanical boundary conditions are formulated just as in classical elasticity theory. The electric boundary conditions are, however, still controversial. The first attempt to define the electric boundary conditions over crack faces was done by Parton [40]. He assumed that although the magnitude of the normal electrical displacement component at the crack face was very small, the electrical displacement was continuous across the crack faces. He used the following electric boundary conditions:Later, Hao and Shen [41] improved the above assumption by taking the electric permeability of air in the crack gap into consideration. In addition to (14), they presented an equation for the boundary condition at crack faces:where is the permittivity of air. However, (15) has remained disregarded for a long time due to its complex mathematical treatment.
As pointed out by Suo et al. [42], the above assumption is not physically practical as there will clearly be a potential drop across the lower capacitance crack. This is particularly true for those piezoelectric ceramics with permittivity 10^{3} times higher than that in the air. For this reason, Deeg [43] proposed another set of electric boundary conditions over crack faces:Equation (16) is derived from the constitutive equation .
This is equivalent to having the crack surfaces free of surface charge which is the electrical boundary condition. Thus the electric displacement vanishes in the environment.
3. ElectromechanicalCoupling Enriched ElementFree Galerkin Method
Displacement and electric potential were adopted as basic field quantities for the solution of the enriched elementfree Galerkin method, and the displacement and electric potential interpolation of a typical point were conducted as follows:where is the MLS shape function at the point . is the support domain. is a set of all nodes whose support is cut by the crack. The set is a set of all nodes that lie within a fixed region around the crack tip. and are the additional degrees of freedom of the displacement. and are the additional degrees of freedom of the electric potential.
The first terms of (15) and (16) are the conventional EFGM approximation which simulates the displacement and electric potential fields. The second term is the displacement and electric potential approximation function of the nodes in . is the Heaviside function:where is the projection of point on the crack.
The last term in (15) and (16) is the displacement and electric potential approximation function of the nodes in . is the branch functions given bywhere and are polar coordinates in the local coordinate system.
The set Ω_{Γ} includes the nodes whose support contains point or is cut by the crack. The set is nodes whose support contains point and crack tip (see Figure 1).
The expression for the potential energy in the domain Ω is given bywhere , , , and are the generalized volume force vector, the given generalized boundary force vector, the generalized boundary displacement vector, and the generalized penalty function coefficient vector, respectively.
In the expressions above,are the generalized strain matrix and generalized elastic matrices.
When the system reaches equilibrium, the potential energy of the system is minimized. The use of the variation principle on (9) and (10) leads to the equilibrium equation:
The standard discrete equations is obtained,
For the enriched terms,and , .
4. A Modified Integral for Functionally Graded Piezoelectric Materials
Owing to the influence of material inhomogeneity in functionally graded piezoelectric materials, the standard integral loses the pathindependence. This section presents a modified integral, which retains the features of the pathindependence.
The integral for piezoelectric material was deduced by Pak [44] aswhere is the electric enthalpy, is an arbitrary contour around the crack, and is the unit outward normal component along path as shown in Figure 2:
Note that the crack is considered to be impermeable and tractionfree.
Numerical determination of the integral is very difficult because the contour, surface, and volume integrals should be defined precisely in the grid. The closed integration path is transformed into an equivalent domain integral (EDI) by applying Gauss’s integral theorem, as can be seen in Figure 3. According to the path independence, (24) could be written aswhere , is an outward normal vector, and is a weighting function which must be continuous and meet the following conditions:
For the functionally graded piezoelectric material, the influence of material inhomogeneity causes the standard integral to lose the characteristic of the pathindependence. A modified integral for calculating the energy release rates of functionally graded piezoelectric material was presented.
Substitute (7) into (17),Let , and (30) is found that where (33) represents the equilibrium equation of the piezoelectric plate whose material constants are the corresponding values at the plane in FGPMs.
From (32) and (33), it can be observed that .
Equations (3)–(6) could be rewritten into Substituting (32)–(35) into (28), it is found thatwhere denotes the integral of the piezoelectric plate whose material constants are the corresponding values at the plane in FGPMs. The standard integral has the characteristic of the pathindependence. So does the .
5. Numerical Example
Case 1. The centrally cracked infinite FGPM plate is shown in Figure 4. The height () and width () are both 0.4 m and the crack length () is 0.02 m. The width of the plate is 20 times the crack length which can be considered to be large enough to simulate an infinite plate with a crack. The positive direction is defined as the polarization direction. The remote uniform distributed stress load is Pa. The remote uniform distributed electric field intensity is V/m. The crack is considered to be permeable and tractionfree. The positive direction is defined as the gradient direction of FGPM. The electron micrograph picture of the crack is shown in Figure 5. The material gradation function: , .
The material properties at were as follows: N/m, N/m, N/m, N/m, N/m, C/m^{2}, C/m^{2}, C/m^{2}, C/V·m, and C/V·m.
As the consequence of the symmetry of the problem, symmetric boundary conditions are imposed; only half of the plate needs to be modeled. In this process, nodes are uniformly distributed in the computational domain, using background grids. In each grid, Gaussian integral and cubic spline weight function are adopted. If a background mesh is present, nodes and the vertices of the integration usually coincide (as in conventional FEM meshes). When cell structures are utilized, a regular array of domains is created, independently of the particle position. It is worth noting that the matrix at a Gauss point is composed of two parts: the standard and the enriched part, where the standard part is always computed and the enriched part is only computed if, in the nodes whose supports cover Gauss point, there exist enriched nodes.
Owing to the existence of additional degrees of freedom, the assembly procedure of stiffness matrix should be revised. Virtual nodes are used to deal with these additional degrees of freedom. One virtual node is added at a Heaviside function enriched node and four virtual nodes are added at a tip enriched node, as depicted in Figure 6. The number of these virtual nodes starts from the total number of true nodes. For example, if there are six nodes numbered from one to six, the third node and fifth node are near tip enriched nodes, and the second node, fourth node, and sixth node are enriched with the Heaviside function. Then, we have nodes. And then we add a virtual node numbered 7 at the second node, add four virtual nodes numbered 8, 9, 10, and 11 at the third node, add a virtual node numbered 12 at the fourth node, add four virtual nodes numbered 13, 14, 15, and 16 at the fifth node, and add a virtual node numbered 17 at the sixth node.
The variation of displacements, and , electric potential, , stresses, and , electric fields, and , and electric displacements, and , are shown in Figure 7. The material property gradient index takes five values: −1, −0.5, 0, 0.5, and 1. As shown in Figure 7, Figure 7(a) presents the displacement of line. Figure 7(b) presents the displacement of line. Figure 7(c) presents electric potential of line. Figure 7(d) presents normal stress of . Figure 7(e) presents normal stress of . Figure 7(f) presents electric field of line. Figure 7(g) presents electric field of line. Figure 7(h) presents electric displacement of line. Figure 7(i) presents electric displacement of line.
(a)
(b)
(c)
(d)
(e)
(f)
(g)
(h)
(i)
For different Gauss integral, the modified integral for FGPM has been computed. The results are listed in Table 1. The largest difference is only 2.08% when compared with the analytical solution which had been obtained from (36). Table 3 illustrates the accuracy of EFGM and EEFGM for calculating the crack of different lengths instead of the different gauss integral.

For a different number of nodes, the modified Jintegrals for FGPM have been computed. , , and nodes are uniformly distributed in the computational domain, using , , and background grids. In each grid, Gaussian integrals are adopted. The results are listed in Table 2. From Table 2, it can be observed that the accuracy of the results by EEFGM has been greatly improved compared with the results by the conventional EFGM.


Case 2. The edgecracked FGPM plate is shown in Figure 8. The height () is 0.4 and the width () is 0.2 m. The crack length () is 0.02 m, 0.04 m, 0.06 m, 0.08 m, and 0.10 m, respectively. The positive direction is defined as the polarization direction. The uniform distributed stress load is Pa. The uniform electric field intensity is V/m. The positive direction is defined as the gradient direction of FGPM. The electron micrograph picture of the crack is shown in Figure 5. The material gradation function: , .
The material properties for PZT5H are as follows: N/m, N/m, N/m, N/m, and N/m; C/m^{2}, C/m^{2}, C/m^{2}, C/V·m, and C/V·m.
In this process, nodes are uniformly distributed in the computational domain, using background grids. In each grid, Gauss integral and cubic spline weight function are adopted.
The modified integral for FGPM has been computed as the crack is under different length. The results are listed in Table 2. The largest difference is only 3% when compared with the analytical solution. From the results listed in Table 2, it can be observed that the Jintegral results obtained by EEFGM have higher accuracy than those calculated by the conventional EFGM.
It is important to note that it can approximately simulate quasistatic crack propagation process with the increase of the crack length.
6. Conclusions
An alternative electromechanicalcoupling enriched elementfree Galerkin method is proposed by introducing extended terms into the approximation function of conventional elementfree Galerkin method to describe the displacement and electric fields near the crack. The major advantage of the present method is that it only needs a small domain to describe the cracktip singular field, and the domain of the node is not affected by the crack. It can improve the computational efficiency without the introduction of the visibility and the diffraction methods, compared with the conventional EFGM. A series of numerical examples for infinite square plate with central cracks of FGPM is solved, and the Jintegrals are calculated. EEFGM has high precision compared with the conventional EFGM with the material property gradient index taking five values. The values of integrals agree well with the analytical solutions. EEFGM can be considered as an alternative numerical method for electromechanicalcoupling problems. It may be potentially attractive for extensions to dynamic fracture analysis of piezoelectric materials.
Conflict of Interests
The authors declare that there is no conflict of interests regarding the publication of this paper.
Acknowledgments
This work was financially supported by the National Natural Science Foundation of China (Grant no. 51305157), the National Key Scientific Instrument and Equipment Development projects, China (Grant no. 2012YQ030075), Jilin Provincial Department of Science and Technology Fund project (Grants nos. 20130305006GX, 201205011, and 201215148), and Graduate Innovation Fund of Jilin University (Project 2015121).
References
 X. Zhu, Q. Wang, and Z. Meng, “A functionally gradient piezoelectric actuator prepared by powder metallurgical process in PNNPZPT system,” Journal of Materials Science Letters, vol. 14, no. 7, pp. 516–518, 1995. View at: Publisher Site  Google Scholar
 B. L. Wang and N. Noda, “Thermally induced fracture of a smart functionally graded composite structure,” Theoretical and Applied Fracture Mechanics, vol. 35, no. 2, pp. 93–109, 2001. View at: Publisher Site  Google Scholar
 S. Ueda, “Thermally induced fracture of a functionally graded piezoelectric layer,” Journal of Thermal Stresses, vol. 27, no. 4, pp. 291–309, 2004. View at: Publisher Site  Google Scholar
 S. Ueda, “A cracked functionally graded piezoelectric material strip under transient thermal loading,” Acta Mechanica, vol. 199, no. 1–4, pp. 53–70, 2008. View at: Publisher Site  Google Scholar
 S. Ueda, “Thermoelectromechanical response of a center crack in a symmetrical functionally graded piezoelectric strip,” Journal of Thermal Stresses, vol. 30, no. 2, pp. 125–143, 2007. View at: Publisher Site  Google Scholar
 S. Ueda, “Effects of crack surface conductance on intensity factors for a functionally graded piezoelectric material under thermal load,” Journal of Thermal Stresses, vol. 30, no. 7, pp. 731–752, 2007. View at: Publisher Site  Google Scholar
 S. Ueda, “Thermal intensity factors for a parallel crack in a functionally graded piezoelectric strip,” Journal of Thermal Stresses, vol. 30, no. 4, pp. 321–342, 2007. View at: Publisher Site  Google Scholar
 C. Li and G. J. Weng, “Antiplane crack problem in functionally graded piezoelectric materials,” Journal of Applied Mechanics, vol. 69, no. 4, pp. 481–488, 2002. View at: Publisher Site  Google Scholar
 K. Q. Hu, Z. Zhong, and B. Jin, “Antiplane shear crack in a functionally gradient piezoelectric layer bonded to dissimilar half spaces,” International Journal of Mechanical Sciences, vol. 47, no. 1, pp. 82–93, 2005. View at: Publisher Site  Google Scholar
 B. N. Rao and M. Kuna, “Interaction integrals for thermal fracture of functionally graded piezoelectric materials,” Engineering Fracture Mechanics, vol. 77, no. 1, pp. 37–50, 2010. View at: Publisher Site  Google Scholar
 A. Borrelli, C. O. Horgan, and M. C. Patria, “Exponential decay of end effects in antiplane shear for functionally graded piezoelectric materials,” Proceedings of the Royal Society of London Series A: Mathematical, Physical and Engineering Sciences, vol. 460, no. 2044, pp. 1193–1212, 2004. View at: Publisher Site  Google Scholar  MathSciNet
 Z. Zhong and E. T. Shang, “Exact analysis of simply supported functionally graded piezothermoelectric plates,” Journal of Intelligent Material Systems and Structures, vol. 16, no. 78, pp. 643–651, 2005. View at: Publisher Site  Google Scholar
 H. L. Dai, Y. M. Fu, and J. H. Yang, “Electromagnetoelastic behaviors of functionally graded piezoelectric solid cylinder and sphere,” Acta Mechanica Sinica, vol. 23, no. 1, pp. 55–63, 2007. View at: Publisher Site  Google Scholar
 H.L. Dai, L. Hong, Y.M. Fu, and X. Xiao, “Analytical solution for electromagnetothermoelastic behaviors of a functionally graded piezoelectric hollow cylinder,” Applied Mathematical Modelling, vol. 34, no. 2, pp. 343–357, 2010. View at: Publisher Site  Google Scholar  Zentralblatt MATH
 Z. Zhong and T. Yu, “Electroelastic analysis of functionally graded piezoelectric material beams,” Journal of Intelligent Material Systems and Structures, vol. 19, no. 6, pp. 707–713, 2008. View at: Publisher Site  Google Scholar
 M. Shakeri and R. Mirzaeifar, “Static and dynamic analysis of thick functionally graded plates with piezoelectric layers using layerwise finite element model,” Mechanics of Advanced Materials and Structures, vol. 16, no. 8, pp. 561–575, 2009. View at: Publisher Site  Google Scholar
 Y. Wang, R. Q. Xu, and H. J. Ding, “Analytical solutions of functionally graded piezoelectric circular plates subjected to axisymmetric loads,” Acta Mechanica, vol. 215, no. 1–4, pp. 287–305, 2010. View at: Publisher Site  Google Scholar
 C. H. Chue and C. N. Yeh, “Angle cracks in two bonded functionally graded piezoelectric material under antiplane shear,” Theoretical and Applied Fracture Mechanics, vol. 53, no. 3, pp. 233–250, 2010. View at: Publisher Site  Google Scholar
 W. Q. Chen and Z. G. Bian, “Wave propagation in submerged functionally graded piezoelectric cylindrical transducers with axial polarization,” Mechanics of Advanced Materials and Structures, vol. 18, no. 1, pp. 85–93, 2011. View at: Publisher Site  Google Scholar
 S. Ueda, “Normal cracks in a functionally graded piezoelectric material strip under transient thermal loading,” Journal of Thermal Stresses, vol. 34, no. 56, pp. 431–457, 2011. View at: Publisher Site  Google Scholar
 I. Ben Salah, Y. Wali, and M. H. B. Ghozlen, “Love waves in functionally graded piezoelectric materials by stiffness matrix method,” Ultrasonics, vol. 51, no. 3, pp. 310–316, 2011. View at: Publisher Site  Google Scholar
 J.S. Wang, X. He, and Q.H. Qin, IUTAM Symposium on Multiscale Modelling of Fatigue, Damage and Fracture in Smart Materials, Springer, 2011.
 C.H. Chue and C.N. Yeh, “Mode III fracture problem of two arbitrarily oriented cracks located within two bonded functionally graded material strips,” Meccanica, vol. 46, no. 2, pp. 447–469, 2011. View at: Publisher Site  Google Scholar  MathSciNet
 M. Enderlein, A. Ricoeur, and M. Kuna, “Finite element techniques for dynamic crack analysis in piezoelectrics,” International Journal of Fracture, vol. 134, no. 34, pp. 191–208, 2005. View at: Publisher Site  Google Scholar  Zentralblatt MATH
 M. Kuna, “Finite element analyses of cracks in piezoelectric structures: a survey,” Archive of Applied Mechanics, vol. 76, no. 1112, pp. 725–745, 2006. View at: Publisher Site  Google Scholar
 E. Béchet, M. Scherzer, and M. Kuna, “Application of the XFEM to the fracture of piezoelectric materials,” International Journal for Numerical Methods in Engineering, vol. 77, no. 11, pp. 1535–1565, 2009. View at: Publisher Site  Google Scholar
 S. S. Nanthakumar, T. Lahmer, and T. Rabczuk, “Detection of multiple flaws in piezoelectric structures using XFEM and level sets,” Computer Methods in Applied Mechanics and Engineering, vol. 275, pp. 98–112, 2014. View at: Publisher Site  Google Scholar  Zentralblatt MATH
 K. Sharma, T. Q. Bui, C. Zhang, and R. R. Bhargava, “Analysis of a subinterface crack in piezoelectric bimaterials with the extended finite element method,” Engineering Fracture Mechanics, vol. 104, pp. 114–139, 2013. View at: Publisher Site  Google Scholar
 A. Bouvier, F. Deleaval, M. M. Doyley et al., “A new finite element method for inverse problems in structural analysis: application to atherosclerotic plaque elasticity reconstruction,” Computer Methods in Biomechanics and Biomedical Engineering, vol. 17, pp. 16–17, 2014. View at: Publisher Site  Google Scholar
 R. R. Ohs and N. R. Aluru, “Meshless analysis of piezoelectric devices,” Computational Mechanics, vol. 27, no. 1, pp. 23–36, 2001. View at: Publisher Site  Google Scholar
 G. R. Liu, K. Y. Dai, K. M. Lim, and Y. T. Gu, “A point interpolation mesh free method for static and frequency analysis of twodimensional piezoelectric structures,” Computational Mechanics, vol. 29, no. 6, pp. 510–519, 2002. View at: Publisher Site  Google Scholar
 T. Y. Ng, H. Li, J. Q. Cheng, K. Y. Lam, and Y. K. Yew, “A novel true meshless numerical technique (hMDOR method) for the deformation control of circular plates integrated with piezoelectric sensors/actuators,” Smart Materials & Structures, vol. 12, no. 6, pp. 955–961, 2003. View at: Publisher Site  Google Scholar
 J. Sladek, V. Sladek, C. Zhang, F. GarciaSanche, and M. Wünsche, “Meshless local PetrovGalerkin method for plane piezoelectricity,” Computers, Materials and Continua, vol. 4, no. 2, pp. 109–117, 2006. View at: Google Scholar
 T. Belytschko, Y. Y. Lu, and L. Gu, “Element‐free galerkin methods,” International Journal for Numerical Methods in Engineering, vol. 37, no. 2, pp. 229–256, 1994. View at: Publisher Site  Google Scholar  MathSciNet
 T. Rabczuk and T. Belytschko, “A threedimensional large deformation meshfree method for arbitrary evolving cracks,” Computer Methods in Applied Mechanics and Engineering, vol. 196, no. 2930, pp. 2777–2799, 2007. View at: Publisher Site  Google Scholar
 T. Rabczuk, P. M. A. Areias, and T. Belytschko, “A simplified meshfree method for shear bands with cohesive surfaces,” International Journal for Numerical Methods in Engineering, vol. 69, no. 5, pp. 993–1021, 2007. View at: Publisher Site  Google Scholar  Zentralblatt MATH
 S. S. Ghorashi, S. Mohammadi, and S.R. SabbaghYazdi, “Orthotropic enriched element free Galerkin method for fracture analysis of composites,” Engineering Fracture Mechanics, vol. 78, no. 9, pp. 1906–1927, 2011. View at: Publisher Site  Google Scholar
 V. P. Nguyen, T. Rabczuk, S. Bordas, and M. Duflot, “Meshless methods: a review and computer implementation aspects,” Mathematics and Computers in Simulation, vol. 79, no. 3, pp. 763–813, 2008. View at: Publisher Site  Google Scholar
 H. Sosa, “On the fracture mechanics of piezoelectric solids,” International Journal of Solids and Structures, vol. 29, no. 21, pp. 2613–2622, 1992. View at: Publisher Site  Google Scholar  Zentralblatt MATH
 V. Z. Parton, “Fracture mechanics of piezoelectric materials,” Acta Astronautica, vol. 3, no. 910, pp. 671–683, 1976. View at: Publisher Site  Google Scholar
 T.H. Hao and Z.Y. Shen, “A new electric boundary condition of electric fracture mechanics and its applications,” Engineering Fracture Mechanics, vol. 47, pp. 793–802, 1994. View at: Google Scholar
 Z. Suo, C.M. Kuo, D. M. Barnett, and J. R. Willis, “Fracture mechanics for piezoelectric ceramics,” Journal of the Mechanics and Physics of Solids, vol. 40, no. 4, pp. 739–765, 1992. View at: Publisher Site  Google Scholar  MathSciNet
 W. F. Deeg, The analysis of dislocation, crack, and inclusion problems in piezoelectric solids [Ph.D. thesis], Stanford University, Stanford, Calif, USA, 1980.
 Y. E. Pak, “Crack extension force in a piezoelectric material,” Transactions ASME, Journal of Applied Mechanics, vol. 57, no. 3, pp. 647–653, 1990. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2015 Guang Wei Meng et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.